Emergence of Magnetism in Doped Two-Dimensional Honeycomb Structures of III–V Binary Compounds
Authors
Open AccessArticle
- First Online:
- Received:
- Accepted:
DOI: 10.1007/s10948-012-1683-1
Abstract
Using first-principles plane-wave calculations, a systematic study of the magnetic properties of doped two-dimensional honeycomb structures of III–V binary compounds has been conducted, both for magnetic or non-magnetic dopants. Calculations show that all cases where the magnetic moment is non-zero are energetically more favorable. For such cases band structure and (partial) density of states were calculated and analyzed in detail. The possible applications of these structures were also discussed.
Keywords
Ab-initio Two-dimensional Magnetism1 Introduction
Since its discovery in 2004 graphene [1] draws much attention because of unique features of this two-dimensional system. Graphene is composed of a sp^{2}-bonded carbon atoms forming a honeycomb structure. It has a very interesting electronic structure with characteristic, linear energy dispersion near K point of the Brillouin zone. A summary of the subject can be found for example in [3].
Shortly after, experimental techniques allowed fabrication of other new two-dimensional materials, like BN and MoS_{2} honeycomb structures [2] or ZnO monolayers [8]. The discovery of such stable two-dimensional material like graphene triggered search for similar structures made from different compounds. Up to now many of these hypothetical structures constructed from silanene (2D Si) and germanene (2D Ge) [4, 5], III–V compounds [6], SiC [7] or ZnO [9] have been studied theoretically.
On the other hand graphene and other nano-scale materials are recognized as future building blocks of new electronics technologies [10], including spintronics (e.g. [11]). In the case of low (one- and two-) dimensional structures problem arises because of famous Mermin–Wagner theorem [12], which prevents ferro- or antiferromagnetic order to occur in finite temperatures, which is essential for spintronics and other modern applications. This started the theoretical and experimental search for magnetism in graphene and other structures. One of the most promising directions is the emergence of magnetism in such structures as an effect of presence of local defects [13]. According to work of Palacios et al. [14] and, independently, of Yazyev [15, 16] single-atom defects can induce ferromagnetism in graphene-based materials. In both cases, the magnetic order arises as an effect of the presence of single-atom defects in combination with a sublattice discriminating mechanism, in agreement with Lieb’s theorem [17, 18]. Based on these findings several theoretical studies have been conducted in search for magnetism in low-dimensional structures either for graphene and BN [19] or other (hypothetical) structures like SiC [7].
In this paper the influence of local defects on magnetic structure of two-dimensional honeycomb structures of GaN, AlN and InN has been analyzed by means of ab-initio calculations. Since bulk versions of these compounds are very important semiconductors in today’s electronics it would be interesting to check whether such two-dimensional materials could have non-zero magnetic moment. Despite of the fact that neither of them have been yet synthesized, calculated cohesion energies [6] suggest that such structures would be stable and their experimental procurement is highly probable.
Next section contains computational details followed by results. Last section concludes this work.
2 Computational Details
To investigate magnetic properties of GaN, AlN and InN honeycomb structures a series of ab-initio calculations have been conducted with use of DFT VASP code [20, 21] with PAW potentials [22]. For both spin-unpolarized and spin-polarized cases the exchange-correlation potential has been approximated by generalized gradient approximation (GGA) using PW91 functional [23]. Kinetic energy cutoff of 500 eV for plane-wave basis set has been used. Supercells of size 3×3×1 have been checked to be large enough to prevent defects to interact with its periodic image.^{1} In all cases for self-consistent structure optimizations, the Brillouin zone (BZ) was sampled by 20×20×1 special k points. All structures have been optimized for both, spin-unpolarized and spin-polarized cases unless Feynman–Hellman forces acting on each atom become smaller than 10^{−4} eV/Å. A vacuum spacing of 12 Å was applied to hinder the interactions between monolayers in adjacent supercells. Calculated lattice constants are in agreement with [6].
3 Results
As mentioned, non-magnetic honeycomb sheets can attain spin-polarized states due to the presence of local defects. In this work two kinds of defects have been analyzed—vacancies and substitutions.
For all three compounds a vacancy was generated first by removing a single atom, Al, Ga, In or N from each supercell, then the atomic structure was optimized. In all cases structures with single N vacancy are non-magnetic, while Al, Ga or In vacancies induce non-zero magnetic moment, equal to 3.00μ _{B}.
Bonding in typical 2D honeycomb structure consists of σ and π states, the former are sp^{2} hybrids while the latter are p_{ z } orbitals. This strong π bonding between two nearest neighbor p_{ z } orbitals makes the structure planar [6]. Covalent σ bonds between adjacent atoms are in-plane.
In the case of AlN (unlike in graphene, [15]) Al vacancy does not break the local threefold symmetry described above. The three adjacent N atoms are left with one dangling bond each, unsaturated, each providing a contribution of magnitude 1μ _{B} to the magnetic moment. In the case of N vacant structures magnetic moment is equal to 0 due to the fact that all electrons in adjacent Al atoms are used to make bond with other N atoms, so there is no unpaired electrons left. Figure 1 shows the density of states (DoS) for spin-polarized Al-vacant AlN, on which difference between majority spin (up) and minority spin (dn) in the vicinity of Fermi level (horizontal line) can be observed which is the main source of non-zero magnetic moment. Analysis of the calculated partial magnetization shows that all magnetic moment is situated on p-states of N atoms located in the area of vacancy.
Magnetic moments and total energy differences between spin up and spin down states for different transition metal elements dopants
AlN | ||||||||||||||
---|---|---|---|---|---|---|---|---|---|---|---|---|---|---|
for Al |
Na |
Mg |
K |
Ca |
Sc |
Ti |
V |
Cr |
Mn |
Fe |
Co |
Ni |
Cu |
Zn |
μ(μ _{B}) |
1.88 |
0.00 |
1.70 |
0.00 |
0.00 |
0.96 |
0.00 |
2.98 |
3.99 |
4.26 |
3.96 |
2.98 |
1.85 |
0.00 |
ΔE (eV) |
0.06 |
0.00 |
0.04 |
0.00 |
0.00 |
0.11 |
0.00 |
0.70 |
0.98 |
1.09 |
0.94 |
0.38 |
0.06 |
0.00 |
GaN | ||||||||||||||
---|---|---|---|---|---|---|---|---|---|---|---|---|---|---|
for Ga |
K |
Ca |
Sc |
Ti |
V |
Cr |
Mn |
Fe |
Co |
Ni |
Cu |
Zn | ||
μ(μ _{B}) |
0.00 |
0.00 |
0.00 |
0.90 |
1.72 |
2.99 |
3.99 |
4.51 |
3.97 |
2.97 |
1.32 |
0.00 | ||
ΔE (eV) |
0.00 |
0.00 |
0.00 |
0.12 |
0.07 |
0.66 |
1.15 |
1.25 |
0.91 |
0.30 |
0.01 |
0.00 |
InN | ||||||||||||||
---|---|---|---|---|---|---|---|---|---|---|---|---|---|---|
for In |
Rb |
Sr |
Y |
Zr |
Nb |
Mo |
Tc |
Ru |
Rh |
Pd |
Ag |
Cd | ||
μ(μ _{B}) |
0.00 |
0.00 |
0.00 |
0.00 |
0.99 |
0.39 |
– |
1.38 |
1.91 |
0.42 |
0.00 |
0.00 | ||
ΔE (eV) |
0.00 |
0.00 |
0.00 |
0.00 |
0.16 |
0.01 |
– |
0.04 |
0.10 |
0.01 |
0.00 |
0.00 |
In the case of doping with alkali metal elements and alkaline earth metal elements only in Na- and K-doped AlN calculations show non-zero magnetic moment (1.88 and 1.70μ _{B}, respectively, for Na and K). The mechanism of formation of magnetic moment is similar to the case of vacant structures (since Na and K have only one valence electron). Figure 2 shows DoS for spin-polarized Na-doped AlN, on which difference between spin up and spin down in the vicinity of Fermi level can be observed.
Magnetic moments and total energy differences between spin up and spin down states for different dopants
AlN | |||
---|---|---|---|
for N |
B |
C |
P |
μ(μ _{B}) |
0.00 |
1.00 |
0.00 |
ΔE (eV) |
0.00 |
0.14 |
0.00 |
GaN | |||
---|---|---|---|
for N |
B |
C |
P |
μ(μ _{B}) |
0.00 |
1.00 |
0.00 |
ΔE (eV) |
0.00 |
0.11 |
0.00 |
InN | |||
---|---|---|---|
for N |
B |
C |
P |
μ(μ _{B}) |
0.00 |
1.00 |
0.00 |
ΔE (eV) |
0.00 |
0.10 |
0.00 |
4 Conclusions
Ab-initio calculations have been conducted for vacancy and substitution defects in honeycomb AlN, GaN and InN compounds. Calculations show that in all three compounds vacancy of Al, Ga or In, respectively, gives magnetic moment of 3.00μ _{B}, which is an interesting conclusion from application point of view. On the other hand substitution of Al or Ga by transition metal elements (Mn, Fe, Co) can give an even higher value of magnetic moment (4.00μ _{B}). Since technique of implantation of metal atoms into 2D surface has been recently reported [24], it is also very promising direction. On the other hand substitution by non-metallic atoms or substitution of nitrogen atoms by IV or V group atoms does not give a significant magnetic moment. These results may give a hint for experimentalists searching two-dimensional magnetic materials.
For chosen structures, calculations within supercell 5×5×1 were conducted, giving the same value of magnetic moment and similar density of states.
Acknowledgements
Numerical calculations were performed at the Interdisciplinary Centre for Mathematical and Computational Modeling (ICM) at Warsaw University.
Open Access
This article is distributed under the terms of the Creative Commons Attribution License which permits any use, distribution, and reproduction in any medium, provided the original author(s) and the source are credited.